Abstract
Quasicrystal structures do not present a full spatial periodicity but are nevertheless constructed starting from deterministic generation rules. When made of different dielectric materials, they often possess fascinating optical properties, which lie between those of periodic photonic crystals and those of a random arrangement of scatterers. Indeed, they can support extended bandlike states with pseudogaps in the energy spectrum, but lacking translational invariance, they also intrinsically feature a pattern of ‘defects’, which can give rise to critically localized modes confined in space, similar to Anderson modes in random structures. If used as laser resonators, photonic quasicrystals open up design possibilities that are simply not possible in a conventional periodic photonic crystal. In this letter, we exploit the concept of a 2D photonic quasi crystal in an electrically injected laser; specifically, we pattern the top surface of a terahertz quantumcascade laser with a Penrose tiling of pentagonal rotational symmetry, reaching 0.1–0.2% wallplug efficiencies and 65 mW peak output powers with characteristic surfaceemitting conical beam profiles, result of the rich quasicrystal Fourier spectrum.
Introduction
Lasing in twodimensional (2D) photonic crystals has been the object of extensive recent research^{1,2,3,4,5}. Operation is normally achieved on modes at the edges of photonic bandgaps or on the localized states formed by suitably designed defects within the periodic photonic lattice. When compared with their periodic counterparts, quasicrystalline structures^{6,7} show significant richness and flexibility in engineering specific device optical properties^{8,9}, like in random structures^{10}. Specifically, the Fourier structure^{11} of quasicrystalline materials, with or without a photonic bandgap, can be exploited in a laser cavity to engineer the mode frequency and spacing separately, or to control the emission profile independently of the feedback conditions. The first reports of quasicrystal lasers made use of optically pumped devices, exploiting either a 2D Penrose lattice^{12,13} or a resonator with 12fold symmetry^{14} and operated at visible frequencies. More recently, the 1D photonic quasicrystal concept has been used with electrically injected THz quantumcascade lasers (QCLs)^{15}, allowing surface emission at chosen angles and wavelengths from tightlyconfining doublemetal waveguides, although the wallplug (WP) efficiency was still poor (≈0.01%)^{15}.
In general, the use of doublemetal waveguides offers considerable advantages for maximizing the operating temperature in THz QCLs, although such devices suffer from the lack of efficient extraction and collimation of the output radiation^{16,17}. These problems have recently been addressed by engineering 1D edgeemitting thirdorder distributed feedback lasers (DFBs)^{18}, 1D photonic heterostructures^{19,20}, 2D annular DFBs^{21} and 2D photonic crystal lasers^{22,23,24}. Using such schemes, vertical surface emission with near zero inplane momentum has been proposed and demonstrated in various implementations, with extraction efficiency values limited by the symmetry of the lasing modes that leads to power cancellations in the farfield. In a periodic structure, indeed, the symmetric and antisymmetric mode feature more than an order of magnitude difference in the quality factor computed including the vertical radiative losses (Q_{vertical}), thereby meaning that lasing results only on the low radiativeefficiency (conventionally named nonradiative), high quality factor modes.
In this letter, we demonstrate that such power cancellation issues can be elegantly circumvented using quasicrystalline resonators, in which the distinction between symmetric (vertically radiative, but low quality factor, Q) and antisymmetric (nonradiative, high Q) modes is fully overcome. In particular, we report the development of high WP efficiency 2D photonic quasicrystal THz QCLs based on a Penrose P2 (kite and dart) tiling with a fivefold rotational symmetry^{6}.
Results
Computational model of the quality factor
The QCL active region^{25} is sandwiched between two metallic cladding layers, to create a doublemetal waveguide that confines, with an almost unitary confinement factor, the THz radiation in the direction of growth (vertical, z axis) and allows its propagation in the x–y plane, therefore making the device a nearly ideal 2D photonic system. To implement the Penrose crystal, holes were opened in the top metallization of a decagonal mesa structure, at the vertices of the Penrose tiles (see Supplementary Fig. 1 and Supplementary Methods), as shown in the scanning electron microscope image of Fig. 1a. The waveguide mode is strongly modified in the hole regions (as the upper metallic cladding layer is missing locally) and radiation can extend outside the semiconductor. Each opening therefore acts not only as a scatterer for the propagating radiation, but also as an aperture through which radiation can be outcoupled. The ratio R between the hole radius r and the spatial length scale a, is maintained between 0.25 and 0.35 to ensure a sufficient degree of scattering/outcoupling, but without overly increasing the waveguide losses and decreasing confinement^{22}. Working with vertical emission, the number of crystal units, chosen here as the smallest one compatible with small mode overlap with the boundaries, controls the lateral confinement of the mode and the ‘probing’ of the absorbing device boundaries and has no influence on the radiative outcoupling.
A full 3D electromagnetic simulation is required to accurately model quasicrystal resonators. While this is possible, it is extremely demanding in terms of computational resources, given the absence of translational invariance and the presence of thin subwavelength metallic layers that require a very fine discretization mesh. As such, we have initially adopted a simplified 2D model^{16}, in which we consider the structure as invariant along the z axis and represented by an equivalent crystal composed of two materials with different local effective dielectric constants (one for the regions comprising the holes, and one for the unpatterned area). The surrounding region is then modelled as an absorbing layer, leading to smooth boundary conditions for the guided modes (see Supplementary Methods). A full 3D simulation was finally performed to have access to the radiative quality factor (Q_{vertical}) and to validate the predictions of the 2D model (see Supplementary Methods).
For the transverse magnetic polarization dictated by the selection rules of intersubband transitions, the opening of complete photonic bandgaps, in an array of low refractive index pillars immersed in a high refractive index material, requires much larger filling factors R than those adopted here. This is even true for periodic crystals^{26}, although it does not preclude lasing at selected kpoints in the lattice reciprocal space where the local density of photonic states (and hence the net gain) is high^{22}. In a band picture, high densities of states are achieved at extremal points where the band dispersion tends to zero and the modes are described by stationary nonpropagating waves. In other words, such states are mainly the result of Bragg reflections from the lattice, coupling counterpropagating modes of wavevectors k and –k, and giving rise to the feedback action necessary for lasing.
Although a band description fails in a quasi crystal owing to the lack of translation invariance, the form factor S(k), obtained as a Fourier transform of the spatial profile of the dielectric constant, still contains relevant information on the main Bragg reflection processes. The Fourier spectrum S(k) of a quasi crystal is indeed often selfsimilar, and, in the limit of large sample size, singular continuous^{13}, meaning that for every two peaks of S(k) there is always a third peak between them. Figure 1b shows the form factor S(k) in reciprocal space for the representative Penrose crystal structure shown in Fig. 1a. While a periodic crystal is characterized by a few welldefined reciprocal wavevectors (Bragg peaks), a quasi crystal has a much richer spectrum with many Bragg resonances (ideally, covering the whole reciprocal space)^{12}. In our Penrose crystal, which contains about 40 spatial units, several main Bragg peaks are present with a characteristic 10fold rotational symmetry^{12}. Standing waves form in the crystal as a consequence of multiple diffractions on the main reciprocal lattice points, according to the relation
where K_{j} are reciprocal lattice Bragg points and k is the optical mode wavevector^{13}.
The quality factor Q of the computed optical modes, quantifying the energy lost per cycle, is plotted in Fig. 1c as a function of radiation frequency for a prototype device with R=0.26 and a=23 μm; this reflects the broad spectrum of Bragg resonances apparent in Fig. 1b, and the lack of photonic bandgaps. A few main modes appear with Q factors significantly higher than the average, and amongst these we identify three dominant modes labelled P, L and H in Fig. 1c that are well within the gain bandwidth of the QCL^{25}. The 2D simulations show that the hole radius and its refractive index both have a strong influence on the Q factor and eigenfrequency of the main optical mode P (see Supplementary Fig. 2). It is worth mentioning that the 2D computed Q_{s} do not contain the radiative contribution Q_{vertical}. As a consequence, they mostly give information on the lateral confinement of the optical modes.
Modes with higher Q factors can here arise only from a reduced overlap with the outer absorbing boundary, that is, from a spatial distribution mainly localized in the device center; these modes are therefore the principal ones confined by the grating feedback. The calculated 2D spatial profiles of P, L and H, represented by the modulus of the electric field component in the vertical (z) direction are shown in Fig. 2a–c, respectively, with their Fourier transforms in reciprocal space shown in Fig. 2d–f (upper left); these present a 10fold symmetry and have peaks at specific values, k_{p}. In the bottomright half of the same panels, the Fourier transform of the spatial profile of the dielectric constant, that is, ε(k) is also plotted.
To identify the Bragg peaks responsible for the feedback, we can overlap the circumferences of circles corresponding to values of nk_{p} that would satisfy eq. (1) for a small finite number of diffractions (for example, n=2 for the simplest twowave coupling k_{p}− K_{j}=−k_{p}, and so on). Their intersections with the relevant points of the reciprocal space, shown in the lower right sections of Fig. 2d–f, indicate which Bragg reflections give rise to the feedback for each mode. The highestQ optical mode, labelled P in Fig. 1c is mainly composed of 10 plane waves, 5 of which are visible in the upper left of Fig. 2d. For this Pmode, the circumference with n=(1+√5)/2, shown in blue in Fig. 2d, intersects strong resonances of S(k), indicating a fivewave diffraction as the origin of feedback. For the lower frequency (L; Fig. 2b) and higher frequency (H; Fig. 2c) modes, clear intersections with the relevant points in S(k) are not found for the main simplest values of n, indicating complex multiple diffraction mechanisms^{13}.
A full 3D simulation was performed to provide an estimate of the photon loss rate due to surface emission γ_{r} (see Supplementary Methods). The vertical radiative losses have been indeed included in the quality factor computation (Q_{vertical}), therefore allowing to have quantitative information on the emission efficiency. The radiative outcoupling efficiency η_{r} is here assumed to be proportional to Q_{total}/Q_{vertical} being Q_{tot}=(1/Q_{inplane}+1/Q_{vertical})^{−1}. The 3D simulations in Fig. 3 show that only one mode, identified with the Pmode, has a total quality factor Q_{tot} significantly above the average, while the relative low Q_{vertical} of the other main modes in Fig. 1c definitely kills their Q_{tot}. From the 3D simulation we extract a Pmode total quality factor Q_{tot}≈147 corresponding to a total photon loss rate γ_{tot}≈21.1 GHz (see Supplementary Methods). The computed Pmode photon loss rate due to surface emission is γ_{r}≈3.4 GHz, corresponding to a Q_{vertical}≈900, and consequently to η_{r}≈16% and to Q_{inplane}≈175, meaning that the main resonator photon loss channel is expected to be the nonradiative inplane one, well supporting the simplified 2D model outcome. It is worth mentioning that there several high frequency modes showing larger η_{r} than the Pmode; however, their significantly lower Q_{tot} (Fig. 3) makes them unable to lase.
Terahertz laser emission in quasicrystal resonators
To realize our devices, the threewell resonantphonon depopulation THz QCL active region of ref. 25 was employed as the gain medium—this structure has a sufficiently wide gain bandwidth so that the main optical mode can be easily tuned by about 13% from the central frequency; this enables the eigenfrequencies of the predicted highQ modes to be tailored within the gain curve. A set of Penroselike 2D resonators having a decagonal section were then fabricated by fixing a=23 μm and varying r in the range 5.8–7.6 μm.
Figure 4a shows the measured current densityvoltage (J–V) and power—current density (L–J) characteristics for four prototype devices with a=23 μm. The threshold current density (J_{th}) slightly varies from 600 to 640 A cm^{−2} as R is changed, with a slope efficiency of 20 mW A^{−1} for the device with R=0.33, which has a peak output power of 8 mW at 10 K under pulsed operation. Figure 4b shows the corresponding laser spectra at J=670 A cm^{−2}. For R=0.33, the quasi crystal supports one main lasing mode at 3.29 THz with an additional smaller intensity peak at a lower frequency (2.84 THz). The main peak red shifts by almost 8 GHz when r is reduced by 7% (R=0.31), a frequency shift smaller than that expected if ones assume the same hole refractive index (≈16 GHz; Supplementary Fig. 2b). In addition, a smaller mode becomes active on the highenergy side. We attribute the main peak for both R=0.33 and R=0.31 to emission from the dominant Pmode of Fig. 1c and Fig. 3, for which a favourable matching with the peak gain of the active material occurs. However, upon further reducing the hole radius to R=0.28 or R=0.26, the Pmode (whose frequency should be further redshifted on the low frequency tail of the gain curve) is no longer visible and a weaker singlemode emission is observed at higher frequencies, associated with the lowerQ modes of Fig. 3, for which a more favourable gain condition is now occurring.
It is worth noticing that, as common in a doublemetal THz QCL, a large portion (around 500 A cm^{−2}) of the threshold injection current is actually due to leakage before the correct band alignment of the structure is reached. As such, threshold current densities only marginally depend on the actual mode Q factor and a reliable determination from the experiments is very difficult to be achieved.
To confirm our interpretation, we fabricated another set of samples with the goal of increasing the Pmode frequency by about 5%. Four devices were tailored with a=22 μm, and r in the range 5.7–7 μm. Figure 4c shows the I–V and L–I characteristics. The peak output power is significantly higher than previously, reaching 45 mW at 10 K for the device with R=0.31, suggesting that P is the main mode responsible for laser emission here. The peak power reduces to 3 mW when the R=0.31 device reaches a heat sink temperature T_{H}=110 K (which corresponds to a lattice temperature of about 148 K).^{27} Owing to the large dissipated electrical power, these devices were not forced to operate at higher currents and temperatures to avoid burnout, therefore hindering a detailed evaluation of the maximum achievable output power and temperatures.
The laser spectra plotted in Fig. 4d for the a=22 μm devices are consistent with our interpretation above. Comparing Fig. 4d,b, we observe that: (i) for R=0.33, the expected 5% shift of the Pmode pushes it out of the material gain curve while a singlemode emission (related to a lowerQ mode) at a lower frequency on the center of the material gain curve is visible; (ii) for R=0.31, the emission is quasi single mode with the main Pmode peak blueshifted by almost 5% with respect to the corresponding peak in Fig. 4b; (iii) for R=0.28, the frequency of the Pmode is now shifted towards the center of the material gain curve and the device can now operate on the Pmode, unlike in Fig. 4b. The recorded frequency is ≈120 GHz less than that observed in the R=0.31 (a=22 μm) sample, a slightly bigger shift than that expected from the 10% radius reduction (which should lead to a 50 GHz frequency drop, see Supplementary Fig. 2b); (iv) for R=0.26, the induced frequency shift is still not enough to induce lasing on the Pmode, which remains on the low frequency side of the material gain curve; the device is therefore still lasing on a lowerQ mode. A final set of devices was fabricated to induce an additional 5% shift in the main mode frequency while keeping the range of filling factors identical (a=21 μm; r=5.4–7.0 μm). The LIV characteristics and spectra are plotted in Fig. 4e,f, respectively. A slight variation in J_{th} is recorded among the devices with different R values. From the spectral analysis we observe that: (i) for R=0.33 and R=0.31, the Pmode is not visible—this is as expected and in line with previous observation. The Pmode is blueshifted too far to the high frequency side of the material gain curve, and is not observed; instead, the device emits on a sequence of modes, blue shifted by almost 5% with respect to the corresponding (R=0.33; 0.31) devices in Fig. 4d; (ii) for R=0.26, emission on the highefficiency Pmode is now observed, in excellent agreement with the prediction of Fig. 3, once the correct ≈10% scaling of the target frequency is taken into account.
It is worth noting that the optical power scales of Fig. 4a,c,e have not been adjusted to take into account both the 78% transmission coefficient of the cyclic olefin cryostat (COC) window and the estimated 90% collection efficiency. If these were included, maximum peak powers of ≈65 mW are achieved, corresponding to a maximum WP efficiency that approaches 0.1%. This is significantly higher than that obtained from more classical geometries such as edgeemitting or dualslit DFB THz QCLs based on the same active region/waveguide combination (Supplementary Fig. 3). Such efficiency performance is also larger than that of conventional periodic structures^{22}. A simple physical explanation is that in quasicrystal resonators the optical modes do not have a naturally defined symmetry of the fields in the aperture.
The surface emission profiles from these devices can be predicted from S(k) and f(k). Any Bragg peak K_{l} existing within the light cone k−k_{p}<2πν/c, centred on k_{p}, allows outofplane scattering, matching the quasicrystal mode with the freespace radiation of inplane wavevector k_{∥}=k_{p}−K_{l}, and frequency ν. The resulting farfield patterns are then composed of a series of spots at given angles, also featuring a 10fold symmetry^{13}. A special case is that of k_{p} being coincident with a given K_{l}: this scattering gives k_{}=0, that is, vertical emission is obtained. This is the case for the Pmode of Fig. 2a,d for which a well collimated emission is expected. A full 3D simulation was performed for this highQ mode, and the farfield pattern was derived from the StrattonChu method applied to the nearfield emission.^{15} Figure 5a shows the simulation results: the beam is collimated into a 8° ring from the vertical and the 10fold symmetry is not apparent. This is expected since the spread of each scattering emission is pointlike only in the limit of an infinite quasi crystal and of a fully spatially coherent optical mode^{13}. In the present case, the modes occupy only a few tens of spatial crystal units, meaning that the preferred angles of emission broaden into more homogeneous ringlike shapes. Figure 5b shows the related experimental measurement. The emission of the quasi crystal (R=0.26, Fig. 4e,f) is well collimated into a ≈10° ring from the vertical with further weaker rings at larger angles, in qualitative agreement with the simulation. Such a ring profile can be converted in a more regular singlelobed pattern by introducing a defect in the central area of the pattern or by grading the hole size across the quasicrystal pattern, that is,. by breaking the resonator rotational symmetry^{23}. For sake of comparison Fig. 5c, shows the angular emission extrapolated for a different sample in which no Pmode emission was detected (R=0.33 in Fig. 4e,f). The emission is here spread in a concentric and more chaotic sequence of rings covering a wider 15° angle, in agreement with the predicted multiple diffraction mechanisms at the origin of the feedback.
Discussion
To make our conclusions more general, we applied the same resonator concept to a different THz QCL active region design (diagonal resonantphoton structure)^{28}, showing a significantly smaller (0.1 THz) gain bandwidth and larger internal quantum efficiency at 3.8 THz. A 0.2% maximum WP efficiency with peak powers of 65 mW has been reached here with similar farfield profiles compatible with Pmode emission. Such efficiency performance is competitive with the best surfaceemitting 1D or 2D THz QCLs resonators (see Supplementary Fig. 4).
In conclusion, we have shown that a 2D photonic quasicrystal concept can be exploited to realize efficient injection lasers based on a quantumcascade active medium in the farinfrared (THz) region of the spectrum. By fabricating a Penrose tiling with pentagonal rotational symmetry in the QCL top metallization layer, highly efficient vertical emission with peak output powers of ≈65 mW and WP in the 0.1–0.2% range can been achieved. Such powers/efficiencies are larger than those achieved with conventional^{22} or uniformly graded 2D photonic crystal lasers^{23} at very low temperatures (4 K), in corresponding doublemetal devices, showing the potential of quasicrystalline structures for the development of more efficient photonic devices and microcavity lasers, as well as for practical metrological and spectroscopy applications across the farinfrared. Furthermore, the described approach may be employed in other physical problems where symmetries need to be broken yet preserving the general order of the system.
Methods
Fabrication procedure
The QCL (sample L341) was grown by molecular beam epitaxy on an undoped GaAs substrate and consists of a GaAs/Al_{0.15}Ga_{0.85}As heterostructure based on the design reported in ref. 25. The growth sequence started with a 250 nm undoped GaAs buffer layer, and was followed by a 300 nm Al_{0.5}Ga_{0.5}As etchstop layer, a 75 nm layer of GaAs ndoped to 5 × 10^{18} cm^{−3}, 226 repetitions of the gain medium creating a 10μm thickness active region, and a final 50 nm GaAs layer ndoped to 5 × 10^{18} cm^{−3}. The thicknesses (in nm) of the active region layers are: 4.8/9.6/2.0/7.4/4.2/16.1, with a 5.6 nm thick portion of the underlined GaAs well being doped to n=5 × 10^{16} cm^{−3} and the Al_{0.15}Ga_{0.85}As barriers being depicted in bold face. After growth, the QCL wafer was thermocompressively bonded with an Au–Au interface on an n^{+}GaAs carrier wafer. After selective removal of the host GaAs substrate by etching, and removing the Al_{0.5}Ga_{0.5}As etchstop layer, the active region was coated with a top Cr/Au (5 nm/150 nm) metallization. Holes of radius r between 5.4–7.7 μm, on a lattice spatial length scale a=23–21 μm, were then lithographically patterned in the metal at each vertex of the Penrose pattern. The 75nm n^{+} contact layer was removed in the holes by reactiveion etching process to reduce the cavity losses. To implement strong absorbing boundary conditions the pattern was surrounded by a predefined thin Cr (7 nm) frame extending 35 μm around the Penrose pattern. This Cr border acted as a mask during the reactiveion etching process, preventing the n^{+} top contact layer from being etched away at the periphery of the Penrose pattern where the absorbing boundary is required. As a final processing step, decagonal mesa structures were etched down to the bottom metal using a H_{2}SO_{4}:H_{2}O_{2}:H_{2}O (11:9:50) etching solution to avoid lateral current spreading. Individual devices were indium soldered onto a copper block and symmetrically wirebonded around the decagon border to ensure uniform current injection through the mesa, while avoiding any perturbative effects in the farfield.
Optical characterization
The lasers were mounted on the cold finger of a heliumflow cryostat, and were driven with 1 μs current pulses at a 1% dutycycle. For the spectral characterization, laser emission was collected with a f/1 parabolic mirror, passed through a Michelson Fourier transform interferometer, and measured in rapid scan with a deuterated triglycine sulfate pyroelectric detector. The light–current curves were measured with a pyroelectric detector at a distance of ≈2.5 cm from the device, without any collection optics and without applying any correction for the cryostat window transmission.
The farfield data were acquired with a pyroelectric detector, which had a sensitive area of about 7 mm^{2} and was mounted at a fixed position. The device was scanned on a x–y translation stage, driven by stepper motors with a spatial resolution of ≈0.2 μm, in the plane perpendicular to the growth direction, at distances of 8 cm and 16 cm from the sample.
Additional information
How to cite this article: Vitiello, M. S. et al. Photonic Quasicrystal Terahertz Lasers. Nat. Commun. 5:5884 doi: 10.1038/ncomms6884 (2014).
References
 1
Meier, M. et al. Laser action from twodimensional distributed feedback in photonic crystals. Appl. Phys. Lett. 74, 7–9 (1999).
 2
Imada, M. et al. Coherent twodimensional lasing action in surfaceemitting laser with triangularlattice photonic crystal structure. Appl. Phys. Lett. 75, 316–318 (1999).
 3
Hirose, K. et al. Wattclass highpower, highbeamquality photoniccrystal lasers. Nat. Photon. 8, 406–411 (2014).
 4
Han, H., Park, H., Cho, M. & Kim, J. THz pulse propagation in plastic photonic crystal fiber. Appl. Phys. Lett. 80, 2634–2636 (2002).
 5
Kakimi, R., Fujita, M., Nagai, M., Ashida, M. & Nagatsuma, T. Capture of a terahertz wave in a photoniccrystal slab. Nat. Photon. 8, 657–663 (2014).
 6
Fujiwara, T. & Ogawa, T. Quasicrystals SpringerVerlag (1990).
 7
Kohmoto, M., Sutherland, B. & Iguchi, K. Localization of optics: quasiperiodic media. Phys. Rev. Lett. 58, 2436–2438 (1987).
 8
Valy Vardeny, Z., Nahata, A. & Agrawal, A. Optics of photonic quasicrystals. Nat. Photon. 7, 177–187 (2013).
 9
Dal Negro, L. & Boriskina, S. V. Deterministic aperiodic nanostructures for photonics and plasmonics applications. Laser Photon. Rev. 5, 1–41 (2011).
 10
Wiersma, D. Disordered photonics. Nat. Photon. 7, 188–196 (2013).
 11
Gumbs, G. & Ali, M. K. Dynamical maps, cantor spectra, and localization for Fibonacci and related quasiperiodic lattices. Phys. Rev. Lett. 60, 1081–1084 (1988).
 12
Kaliteevski, M. A. et al. Penrosetiled photonic quasicrystals: from diffraction pattern to band structure. Nanotechnology 11, 274–280 (2000).
 13
Notomi, M., Suzuki, H., Tamamura, T. & Edagawa, K. Penroselattice photonic quasicrystal laser. Phys. Rev. Lett. 92, 123906 (2004).
 14
Nozaki, K. & Baba, T. Quasiperiodic photonic crystal microcavity lasers. Appl. Phys. Lett. 84, 4875–4877 (2004).
 15
Mahler, L. et al. Quasiperiodic distributed feedback laser. Nat. Photon. 4, 165–169 (2010).
 16
Mahler, L. & Tredicucci, A. Photonic engineering of surfaceemitting terahertz quantum cascade lasers. Laser Photon. Rev. 5, 647–658 (2011).
 17
Sirtori, C., Barbieri, S. & Colombelli, R. Wave engineering with THz quantum cascade lasers. Nat. Photon. 7, 691–701 (2013).
 18
Amanti, M. I., Fischer, M., Scalari, G., Beck, M. & Faist, J. Lowdivergence singlemode terahertz quantum cascade laser. Nat. Photon. 3, 586–590 (2009).
 19
Xu, G. et al. Efficient power extraction in surfaceemitting semiconductor lasers using graded photonic heterostructures. Nat. Commun. 3, 952 (2012).
 20
Xu, G. et al. Surfaceemitting terahertz quantum cascade lasers with continuouswave power in the tens of milliwatt range. Appl. Phys. Lett. 104, 091112 (2014).
 21
Liang, G. et al. Low divergence singlemode surfaceemitting concentriccirculargrating terahertz quantum cascade lasers. Opt. Express 21, 31872–31882 (2013).
 22
Chassagneux, Y. et al. Electrically pumped photoniccrystal terahertz lasers controlled by boundary conditions. Nature 457, 174–178 (2009).
 23
Chassagneux, Y. et al. Graded photonic crystal terahertz quantum cascade lasers. Appl. Phys. Lett. 96, 031104 (2010).
 24
Halioua, Y. et al. THz quantum cascade lasers operating on the radiative modes of a 2D photonic crystal. Opt. Lett. 39, 3962–3965 (2014).
 25
Belkin, M. A. et al. Terahertz quantum cascade lasers with copper metalmetal waveguides operating up to 178 K. Opt. Express 13, 3242–3248 (2008).
 26
Joannopoulos, J. D., Johnson, S. G., Winn, J. N. & Meade, R. D. Photonic Crystals: Molding the Flow of Light Princeton Univ. Press (2008).
 27
Vitiello, M. S. et al. Thermal properties of THz quantum cascade lasers based on different optical waveguide configurations. Appl. Phys. Lett. 89, 021111 (2006).
 28
Kumar, S., Hu, Q. & Reno, J. L. 186 K operation of terahertz quantumcascade lasers based on a diagonal design. Appl. Phys. Lett. 94, 131105 (2009).
Acknowledgements
This work was partly supported by the Italian Ministry of Education, University, and Research (MIUR) through the programme ‘FIRB—Futuro in Ricerca 2010 RBFR10LULP ‘Fundamental research on Terahertz photonic devices’, the EPSRC (UK) and the ERC program ‘TOSCA’ and ‘SouLMan’. We also acknowledge the support of the Royal Society and the Wolfson Foundation. We thank D. Wiersma and R. Colombelli for useful discussion.
Author information
Author notes
Affiliations
Contributions
M.S.V., A.T and A.R. devised the concept; A.R., F.C. and V.T. performed the simulations; M.N. fabricated the devices; M.S.V. and M.N. performed the experiments; L.L., E.H.L. and A.G.D. carried out the growth of QCL materials; M.S.V. analysed the data; M.S.V. wrote the manuscript with the contributions from the other authors. M.S.V. and A.T. coordinated the whole project.
Corresponding author
Correspondence to Miriam Serena Vitiello.
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures 14, Supplementary Methods and Supplementary References (PDF 1028 kb)
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Vitiello, M., Nobile, M., Ronzani, A. et al. Photonic quasicrystal terahertz lasers. Nat Commun 5, 5884 (2014) doi:10.1038/ncomms6884
Received
Accepted
Published
DOI
Further reading

Robust transmission of orbital angular momentum mode based on a dualcladding photonic quasicrystal fiber
Journal of Physics D: Applied Physics (2019)

Refractive index sensing characteristics in a Dshaped photonic quasicrystal fiber sensor based on surface plasmon resonance
Journal of the Optical Society of America A (2019)

Scattering strength dependence of terahertz random lasers
Journal of Applied Physics (2019)

Octonacci magnetophotonic quasicrystals
Optical Materials (2019)

Frequencytunable continuouswave random lasers at terahertz frequencies
Light: Science & Applications (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.